- Open Access
Interfacial biomechanical properties of a dual acid-etched versus a chemically modified hydrophilic dual acid-etched implant surface: an experimental study in Beagles
© The Author(s). 2018
- Received: 1 February 2018
- Accepted: 29 May 2018
- Published: 27 September 2018
The high survival clinical success rates of osseointegration are requisites for establishing a long-term biomechanical fixation and load-bearing potential of endosseous oral implants. The objective of this preclinical animal study was to evaluate the effect of surface microtopography and chemistry on the early stages of biomechanical rigidity with a sandblasted, dual acid-etched surface, with or without an additional chemical modification (SAE-HD and SAE, respectively), in the tibia of Beagle dogs.
Two pairs of implants, with the same macrogeometry but different surface technology ((a) dual acid-etched surface treatment with hydrochloric and sulfuric acid followed by microwave treatment and insertion in isotonic saline solution to increase hydrophilicity (SAE-HD) (test, n = 12) and (b) dual acid-etched surface (SAE) (control, n = 12)), were installed bilaterally in the proximal tibia of six Beagle dogs. In order to determine the effect of surface modification on biomechanical fixation, a test protocol was established to assess the torque and a complete set of intrinsic properties. Maximum removal torque (in N cm) was the primary outcome measure, while connection stiffness (N cm/rad) and removal energy (× 10−2J) were the secondary outcome measures and were assessed after 2 and 4 weeks in vivo. A general linear statistical model was used and performed for significant differences with the one-way ANOVA followed by Tukey post hoc test (P < 0.05).
The removal torque values did not reveal significant statistical differences between SAE-HD and SAE implants at any observation times (P = 0.06). Although a slight increase over time could be observed in both test and control groups. SAE-HD showed higher removal energy at 4 weeks (999.35 ± 924.94 × 10− 2 J) compared to that at 2 weeks (421.94 ± 450.58 × 10− 2 J), while SAE displayed lower values at the respective healing periods (P = 0.16). Regarding connection stiffness, there were no significant statistical differences neither within the groups nor over time. There was a strong, positive monotonic correlation between removal torque and removal energy (=0.722, n = 19, P < 0.001).
In this study, no significant differences were observed between the specific hydrophilic (SAE-HD) and hydrophobic (SAE) surfaces evaluated, in terms of biomechanical properties during the early osseointegration period.
- Dental implant
- Removal torque
- Removal energy
- Connection stiffness
- Implant roughness
- New methodology assessment for implants
The progressive evolution of oral implant surface technology (i.e., micro to nanotopography and chemical composition) [1, 2], implant macrogeometry, surgical procedures [3–5], and loading protocols [6–8] has resulted in high survival and clinical success rates . Accordingly, chemically active micro and nanostructured implant surfaces, presenting moderate surface roughness (Ra/Sa values between 1 and 2 μm), enhance host-to-implant interactions [10–12] and have been shown to shorten the period needed for time-critical functional implant loading (i.e., so-called immediate or early loading) [13–15].
Recent in vitro analyses support the concept that hydrophilic surfaces upregulate the expression of angiogenic factors, activate the production of anti-inflammatory factors, and downregulate the expression of pro-inflammatory cytokines by osteoblasts  and macrophage-like cells [17, 18], and regulate osteogenic differentiation and maturation of mesenchymal stem cells (MSCs) [10, 19, 20] and human osteoblast-like cells [21–23], increasing osteogenesis and decreasing osteoclastogenesis [11, 23, 24]. Furthermore, higher surface energy and hydrophilicity is demonstrated to induce faster bone-to-implant contact (%BIC) and bone density, both in preclinical in vivo experiments [25–27] and in patients [7, 28, 29]. Indeed, higher biomechanical stability as expression of primary and secondary bone anchorage is recorded following hydrophilic implant placement [26, 30].
Particularly, a superhydrophilic moderately rough titanium (Ti) implant surface (contact angle less than 5°) has been suggested to play a critical role during the early healing period  and establishment of a successful osseointegration  in preclinical in vivo studies. The microarchitecture and density of the trabecular bone formed around oral implants, characterized by a high ratio of metabolic activity and remodeling, is one of the main determinants of interfacial shear strength, mechanical resistance, and adaptation to overloading stress . The potential of chemically modified superhydrophilic implant surfaces to enhance osteogenic differentiation and increase early bone apposition onto the implant may shorten the implant stability drop, occurring due to bone remodeling during the first few weeks of implantation . Consequently, such microstructured surface technology may lessen the healing (non-loading) period and allow more readily immediate or early functional implant loading in patients with reduced bone density. Nevertheless, there is lack of knowledge regarding the intrinsic biomechanical aspects of osseointegration related to this specific implant surface technology (i.e., removal torque, removal energy, and connection stiffness) during the initial osseointegration process.
Evaluation of biological effects and biomechanical properties of innovative technologies in the field of implant dentistry in preclinical animal models, prior to translational research, complies with standard regulations . Thus, the aim of this preclinical animal study was to evaluate the effect of surface microtopography and chemistry on the biomechanical properties of implants with a sandblasted, dual acid-etched surface, with or without an additional chemical modification (SAE-HD1 and SAE,2 respectively), during the early stages of osseointegration in the tibia of Beagle dogs. Specifically, we hypothesized that a chemically active implant surface presenting superhydrophilicity generates higher interfacial shear strength in comparison to a hydrophobic surface, expressed as higher maximum removal torque, removal energy, and connection stiffness.
The present preclinical in vivo study is reported according to the Animal Research: Reporting of In Vivo Experiments (ARRIVE) guidelines, in regard with relevant items . The animal experimental protocol was approved by the Bioethics Committee for Animal Experimentation (CEUA, protocol no. 098/10) at the Federal University of Uberlândia and followed the normative guidelines of the National Council for Animal Control and Experimentation (CONCEA), constituent of the Ministry of Science, Technology and Innovation (MCTI), Law no. 11.794, 08/19/2008, Brazil. The in vivo part of the study was conducted between November 2012 and January 2013.
Twenty-four commercially pure Ti implants (10 mm × 4 mm, L × Ø) with a moderately rough surface, produced by means of sandblasting and dual acid-etching with hydrochloric and sulfuric acid were used in the present study. Implants in the control group were only sandblasted and dual acid-etched (SAE; n = 12). In the test group, after sandblasting and dual acid etching, implants received proprietary technology treatment, including microwave treatment and insertion in isotonic saline solution resulting in significantly increased hydrophilicity (SAE-HD; n = 12). These specific implant surfaces exhibit the following 3D surface roughness parameters for SAE and SAE-HD, respectively: Sa 1.44 μm ± 1.15 and 1.26 μm ± 0.17; Sz 14.57 μm ± 1 and 16.20 μm ± 7.8; Sdr 1.51 and 1.21%; Sds 658.67 1/mm2 ± 27.42 and 643.33 1/mm2 ± 37.74; and Ssk −0.51 and −0.43 . The chemical composition of the different surfaces was examined by X-ray photoelectron spectroscopy (XPS). The atomic percentage values of carbon were 49 and 17, and 22 and 59 of oxygen in SAE and SAE-HD groups, respectively. The surface energy and wettability was investigated by means of a static contact angle analysis by means of the sessile drop technique  applying simulated body fluid (SBF) solution. SAE-HD disks reveal a superhydrophilic behavior (contact angle < 5°), whereas SAE surfaces display superhydrophobic properties (contact angle > 90°).
The implants present similar macrodesign with an external hexagon connection system and cylindrical body containing double triangular threads with high potential for bone compression recommended for type III and IV bone, commercially available as Titamax Ti Ex®. Neodent®3 supplied all implants.
Six male Beagle dogs (~ 1.5 years old), weighting between 13 and 15 kg, were used in the present study. All animals were acclimatized in the experimental animal care facility of Federal University of Uberlândia for 2 weeks previously to the experimental procedures and randomly pair-housed in standard shelters (1 × 1.5 m kennel) to allow environmental enrichment (i.e., variety of toys, daily group play sessions, resistance running, and training) at the ambient temperature of 22 °C, under controlled humidity and 12-h circadian rhythm. The diet consisted of hard pellet and water ad libitum. The animal caretakers were blind to the experimental groups. The level of pain, distress, or suffering was daily assessed during the observation period to ensure the welfare of the animals. Aiming to guarantee selection blindness during the experimental allocation, the groups were systematically coded by a third person and the first implant to be placed in each tibia was randomly assigned. Sample size was calculated based on information in previous studies using the dog tibia model to allow evaluation of possible differences in bone-to-implant contact between groups. The surgical procedures and the histological/histomorphometrical outcomes of the study have been reported elsewhere .
Assessment of interfacial biomechanical properties
To assess the biomechanical strength of the bone-implant interface, the following parameters were assessed: (a) maximum removal torque (N cm) (primary outcome measure), obtained during the unscrewing process (primary outcome measure); (b) connection stiffness (N cm/rad), corresponding to the ratio between removal torque and angular displacement (secondary outcome measure); and (c) removal energy (× 10–2 J), corresponding to the energy (workload) necessary to completely unscrew the implant (secondary outcome measure).
Calibration of one blinded examiner (R.N.R.J) and repeated measurements for data reproducibility was performed under supervision and prior to performing the removal torque test and respective calculation of connection stiffness.
A general linear statistical model with torque, energy, and stiffness as dependent variables and implant surface and time in vivo as independent variables was used at 95% level of significance and performed by one-way ANOVA followed by Tukey’s post hoc test. The Spearman rank correlation test was taken in order to test the association concerning the investigated dependent variables. Since sample size calculation, as already mentioned, was made to allow evaluation of possible differences in bone-to-implant contact between groups, a post hoc analysis was performed to define the minimum detectable difference between groups regarding the parameters assessed herein, with a power of 80% and an alpha error of 0.05%. The IBM® SPSS® Statistics software5 was used.
One-way ANOVA variance and Tukey’s post hoc test values of removal torque (N cm), removal energy [N cm/rad (0.01 J)], and connection stiffness [N cm/rad] for SAE-HD and SAE implants at 2 and 4 weeks postoperatively (n = 6; P < 0.05)
Sum of squares
Sig. (P value)
The removal torque values (N cm) did not reveal significant statistical differences between SAE-HD and SAE implants at any observation period (P = 0.06), but a slight increase over time could be observed in both test and control groups (Fig. 5a). Removal torque at 2 weeks was 60.18 ± 24.12 and 54.00 ± 29.91 N cm, and at 4 weeks was 88.11 ± 14.96 and 79.05 ± 14.59 N cm for SAE-HD and SAE implants, respectively (Fig. 5b). SAE-HD showed higher removal energy [J] at 4 weeks (9.99 ± 9.25) compared to 2 weeks (4.22 ± 4.50), while SAE displayed lower values at corresponding healing times (5.21 ± 1.49 vs. 2.83 ± 2.49, respectively) (P = 0.16). Regarding connection stiffness (N cm/rad), SAE showed lower values at 2 weeks (462.57 ± 507.75) compared with 4 weeks of healing (689.01 ± 496.28), however not statistically significant (Fig. 5c). SAE-HD disclosed similar results at 2 and 4 weeks (652.98 ± 111.26 vs. 661.56 ± 369.28, respectively) without statistically significant differences neither between the groups, nor over time (P = 0.76).
Spearman rank correlation coefficient values between removal torque (N cm), removal energy [N cm/rad (0.01 J)], and connection stiffness [N cm/rad] for SAE-HD and SAE implants at 2 and 4 weeks postoperatively (n = 6; P < 0.01)
Improving surface wettability aims to increase the implant surface area achieving most favorable protein adsorption and cellular adhesion and thereby to positively regulate the biological response at the initial osseointegration process. Thus, the superior potential of superhydrophilic surfaces in enhancing osseointegration at early stages of bone formation may also enhance their load-bearing capacity and biomechanical resistance.
In the present study, both SAE-HD implants and SAE implants showed relatively high amounts of maximum removal torque values at both observation times. In contrast, the SAE-HD implants showed relatively high values in removal energy compared with SAE implants at both 2 and 4 weeks. Specifically, the test group presented consistently higher values (about 100% higher) in removal energy compared with the control group at both observation times. Further, SAE-HD implants showed high values in connection stiffness already after 2 weeks of healing, while SAE implants required 4 weeks of healing to reach a similar level. Thus, despite the fact that the differences between the two groups were not significant for any of the evaluated parameters or observation times, the results seem to indicate that differences in surface properties between SAE-HD and SAE implants, somehow influenced osseointegration and intrinsic properties of shear strength. Indeed, greater removal torque values and interfacial stiffness for hydrophilic implants (modSLA)1 between 2 and 4 weeks, in comparison with SLA2, have been previously reported . In this study , performed in the anterior maxilla of miniature pigs, hydrophilic implants revealed, on average, 8–21 and 9–14% significantly higher removal torque and interfacial stiffness values, respectively, than those of the SLA implants. Due to the remodeling process, the biomechanical parameters decreased with time for both implant surfaces, reflecting the developing biological stability.
It has been previously reported the existence of a correlation between removal torque and %BIC values , although the nature of these parameters differs from one another (three-dimensional versus most often two-dimensional parameter) . Indeed, the lack of differences between the groups herein reflect well the results of the histomorphometric analysis of the other half of implants in the present study, reported elsewhere . In particular, similar amounts of osseointegration in terms of %BIC and bone density were observed in both groups (SAE-HD vs. SAE) at each observation time, and there were no statistically significant differences regarding the respective parameters between the two observations times . In contrast, Sartoretto et al.  demonstrated that Acqua® implants (Neodent®), which present similar technology as the SAE-HD implants, resulted in accelerated osseointegration when placed in tibia of rabbits after 2 weeks of healing, compared with implants with the Neoporos® surface, which in turn presents similar technology with the SAE surface. The difference between the study of de Jesus et al.  and Sartoretto et al.  in terms of the impact of surface technology on histomorphometric osseointegration parameters may be due to anatomical and/or biological differences in the experimental models employed. In this context, although there is no scientific support regarding the optimal experimental model to evaluate aspects of osseointegration, the dog is one of the most commonly used animal platforms . The mandible of dogs is the most frequent location; however, a high percentage of studies on implant integration have used extra-oral implant sites, including the tibia . It is suggested that due to its anatomy, with a large lumen and relatively low trabecular density , it possesses high discriminating potential regarding the impact of implant surface technologies to enhance osseointegration. Furthermore, the tibia allows placement of a larger number of implants comparing with the mandible, thus allowing the use of fewer animals and/or multiple types of comparisons/tests (e.g., biomechanical and histological evaluation).
On the other hand, lack of significant differences between the two groups in the present experiment could be due to the fact that the effect of hydrophilicity, in terms of accelerating bone healing and osseointegration, was unfolded before the first evaluation time-point of 2 weeks, i.e., during the very early healing period. Consistently, pre-clinical investigations show the potential of chemically modified surfaces to rapidly modulate the host-to-implant response upon prompt adsorption of blood proteins [20, 22]. In a recent study reported by Vasak et al. , hydrophilic implants (SLActivea) strengthened the apposition of newly formed bone at the very early healing period between 5 and 10 days in the intra-oral model of minipigs, even though they did not reveal significant statistical differences in comparison to hydrophobic surfaces (SLA). Clinically, a systematic review of human histological studies on molecular aspects of osseointegration  has shown that moderately rough implant surfaces with high hydrophilicity enhance molecular processes related to osseointegration during the early stages of wound healing. Similar clinical studies assessed the degree of new bone-to-implant contact (%NBIC) around SLActive implants in comparison to SLA placed in the mandibular retromolar region in man during the early stages of osseointegration [28, 40]. The authors reported a progressive increase in %NBIC around both implants, whereas chemically active surfaces disclosed higher values at 2 and 4 weeks compared with SLA, no longer observed after 6 weeks of osseointegration.
Studies including biomechanical analysis of osseointegration are usually assessing maximum removal torque. Although this parameter is important, use of a single parameter appears not sufficient for a complete biomechanical assessment of osseointegration. Herein, connection stiffness, reflecting the rigidity (i.e., the stability of the implant under load), and removal energy, reflecting the overall energy (workload) necessary to loosen the bone-to-implant connection, were additionally assessed. It is suggested that the use of these three parameters in a complementary manner is essential for complete evaluation of the biomechanical properties of implants. Indeed, two different osseointegrated implants can have the same maximum removal torque, but distinct connection stiffness; similarly, they may show the same removal energy but perform in a very distinct fashion and show distinct connection stiffness and maximum removal torque. To the best of the authors’ knowledge, this is the first original research reporting removal energy as an intrinsic removal torque property in relation to connection stiffness during biomechanical assessment of hydrophilic implants; however, removal energy has already been used assessing mini-implants with hydrophobic surfaces .
In fact, the observed lack of differences between the groups could be attributed to the relatively low number of specimens per group. According to the observed data herein, applying a high power (80%) with the present sample size would had revealed a relatively large difference in removal torque equivalent to 43% between the experimental groups. Regarding removal energy and connection stiffness, this difference would had been equal to 71 and 34%, respectively. In addition, a significant difference may not had been achieved due to the nature of the specimens. Biological material properties vary greatly from organism to organism and even in the same animal. Therefore, in future studies when using the presented methodology, a greater number of specimens must be considered. This will evidence a superior discrimination capacity. Nonetheless, the current methodology is far more reliable than the use of a single parameter methodology.
No significant differences were observed between the specific hydrophilic (SAE-HD) and hydrophobic (SAE) surfaces evaluated in this study, in terms of biomechanical properties during the early osseointegration period.
Chemically modified sandblasted, large grit, and acid-etched surfaces
Sandblasted, large grit, and acid-etched surfaces
Neodent, Rua Benjamin Lins, 742, Curitiba, PR 80420–100, Brazil
Shimadzu Corporation, Nishinokyo Kuwabara-cho, Nakagyo-ku, Kyoto 604–8511, Japan
IBM Corporation v.23, 1 New Orchard Road, Armonk, New York 10, 504–1722, USA
The assistance of fifth-year dental students of the Federal University of Uberlândia in surgeries, including auscultation, and other practicalities is highly appreciated.
The Brazilian Federal Agency for Support and Evaluation of Graduate Education (CAPES research fellow, Full PhD Program, process no. 0975-14.1) provided funding and Neodent® (Curitiba, PR, Brazil) produced the titanium implants. None of the funding institutions influenced the study design and data collection, analysis, and interpretation or the manuscript writing process.
Availability of data and materials
The datasets used and/or analyzed during the current study are available from the corresponding author on reasonable request.
RNRJ participated in the study concept and design and performed the animal operations, biomechanical test, and data analysis and interpretation. EC, PVA, and AR contributed to define the test protocol and performed the biomechanical test and data analysis. CCGM and DZ participated in the study concept and design and performed the animal operations and data analysis. AS contributed to data analysis, interpretation, and drafting of the manuscript. All authors have contributed to and/or critically revised the manuscript and given approval to the final version of the manuscript.
The animal experimental protocol was approved by the Bioethics Committee for Animal Experimentation (CEUA, protocol no. 098/10) at the Federal University of Uberlândia.
Rainde Naiara Rezende de Jesus, Eunice Carrilho, Pedro V. Antunes, Amílcar Ramalho, Camilla Christian Gomes Moura, Andreas Stavropoulos, and Darceny Zanetta-Barbosa declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Cochran DL, Jackson JM, Jones AA, Jones JD, Kaiser DA, Taylor TD, et al. A 5-year prospective multicenter clinical trial of non-submerged dental implants with a titanium plasma-sprayed surface in 200 patients. J Periodontol. 2011;82(7):990–9. https://doi.org/10.1902/jop.2011.100464.View ArticlePubMedGoogle Scholar
- Wallkamm B, Ciocco M, Ettlin D, Syfrig B, Abbott W, Listrom R, et al. Three-year outcomes of Straumann Bone Level SLActive dental implants in daily dental practice: a prospective non-interventional study. Quintessence Int. 2015;46(7):591–602. https://doi.org/10.3290/j.qi.a34076. PubMedGoogle Scholar
- Baires-Campos FE, Jimbo R, Bonfante EA, Fonseca-Oliveira MT, Moura C, Zanetta-Barbosa D, et al. Drilling dimension effects in early stages of osseointegration and implant stability in a canine model. Med Oral Patol Oral Cir Bucal. 2015;20(4):471–9.View ArticleGoogle Scholar
- Blanco J, Alvarez E, Munoz F, Linares A, Cantalapiedra A. Influence on early osseointegration of dental implants installed with two different drilling protocols: a histomorphometric study in rabbit. Clin Oral Implants Res. 2011;22(1):92–9. https://doi.org/10.1111/j.1600-0501.2010.02009.View ArticlePubMedGoogle Scholar
- Jimbo R, Tovar N, Anchieta RB, Machado LS, Marin C, Teixeira HS, et al. The combined effects of undersized drilling and implant macrogeometry on bone healing around dental implants: an experimental study. Int J Oral Maxillofac Surg. 2014;43(10):1269–75. https://doi.org/10.1016/j.ijom.2014.03.017.View ArticlePubMedGoogle Scholar
- Marković A, Čolić S, Šćepanović M, Mišić T, Ðinić A, Bhusal DS. A 1-year prospective clinical and radiographic study of early-loaded bone level implants in the posterior maxilla. Clin Implant Dent Relat Res. 2015;17(5):1004–13. https://doi.org/10.1111/cid.12201.View ArticlePubMedGoogle Scholar
- Nicolau P, Korostoff J, Ganeles J, Jackowski J, Krafft T, Neves M, et al. Immediate and early loading of chemically modified implants in posterior jaws: 3-year results from a prospective randomized multicenter study. Clin Implant Dent Relat Res. 2013;15(4):600–12. https://doi.org/10.1111/j.1708-8208.2011.00418. View ArticlePubMedGoogle Scholar
- Romanos G, Grizas E, Laukart E, Nentwig GH. Effects of early moderate loading on implant stability: a retrospective investigation of 634 implants with platform switching and Morse-tapered connections. Clin Implant Dent Relat Res. 2016;18(2):301–9. https://doi.org/10.1111/cid.12314.View ArticlePubMedGoogle Scholar
- Karabuda ZC, Abdel-Haq J, Arιsan V. Stability, marginal bone loss and survival of standard and modified sand-blasted, acid-etched implants in bilateral edentulous spaces: a prospective 15-month evaluation. Clin Oral Implants Res. 2011;22(8):840–9. https://doi.org/10.1111/j.1600-0501.2010.02065. View ArticlePubMedGoogle Scholar
- Wall I, Donos N, Carlqvist K, Jones F, Brett P. Modified titanium surfaces promote accelerated osteogenic differentiation of mesenchymal stromal cells in vitro. Bone. 2009;45(1):17–26. https://doi.org/10.1016/j.bone.2009.03.662.View ArticlePubMedGoogle Scholar
- Mamalis AA, Markopoulou C, Vrotsos I, Koutsilirieris M. Chemical modification of an implant surface increases osteogenesis and simultaneously reduces osteoclastogenesis: an in vitro study. Clin Oral Implants Res. 2011;22(6):619–26. https://doi.org/10.1111/j.1600-0501.2010.02027. View ArticlePubMedGoogle Scholar
- Lotz EM, Olivares-Nasarrete R, Berner S, Boyan BD, Schwartz Z. Osteogenic response of human MSCs and osteoblasts to hydrophilic and hydrophobic nanostructured titanium implant surfaces. J Biomed Mater Res A. 2016;104(12):3137–48. https://doi.org/10.1002/jbm.a.35852.View ArticlePubMedGoogle Scholar
- Chambrone L, Shibli JA, Mercurio CE, Cardoso B, Preshaw PM. Efficacy of standard (SLA) and modified sandblasted and acid-etched (SLActive) dental implants in promoting immediate and/or early occlusal loading protocols: a systematic review of prospective studies. Clin Oral Implants Res. 2015;26(4):359–70. https://doi.org/10.1111/clr.12347.View ArticlePubMedGoogle Scholar
- Heinemann F, Hasan I, Bourauel C, Biffar R, Mundt T. Bone stability around dental implants: treatment related factors. Ann Anat. 2015;199:3–8. https://doi.org/10.1016/j.aanat.2015.02.004.View ArticlePubMedGoogle Scholar
- Hinkle RM, Rimer SR, Morgan MH, Zeman P. Loading of titanium implants with hydrophilic endosteal surface 3 weeks after insertion: clinical and radiological outcome of a 12-month prospective clinical trial. J Oral Maxillofac Surg. 2014;72(8):1495–502. https://doi.org/10.1016/j.joms.2014.04.016.View ArticlePubMedGoogle Scholar
- Hyzy SL, Olivares-Navarrete R, Hutton DL, Tan C, Boyan BD, Schwartz Z. Microstructured titanium regulates interleukin production by osteoblasts, an effect modulated by exogenous BMP-2. Acta Biomater. 2013;9(3):5821–9. https://doi.org/10.1016/j.actbio.2012.10.030.View ArticlePubMedGoogle Scholar
- Hamlet S, Alfarsi M, George R, Ivanovski S. The effect of hydrophilic titanium surface modification on macrophage inflammatory cytokine gene expression. Clin Oral Implants Res. 2012;23(5):584–90. https://doi.org/10.1111/j.1600-0501.2011.02325. View ArticlePubMedGoogle Scholar
- Hotchkiss KM, Ayad NB, Hyzy SL, Boyan BD, Olivares-Navarrete R. Dental implant surface chemistry and energy alter macrophage activation in vitro. Clin Oral Implants Res. 2017;28(4):414–23. https://doi.org/10.1111/clr.12814.View ArticlePubMedGoogle Scholar
- Rosa AL, Kato RB, Castro Raucci LMS, Teixeira LN, de Oliveira FS, Bellesini LS, et al. Nanotopography drives stem cell fate toward osteoblast differentiation through α1β1 integrin signaling pathway. J Cell Biochem. 2014;115(3):540–8. https://doi.org/10.1002/jcb.24688.View ArticlePubMedGoogle Scholar
- Boyan BD, Cheng A, Olivares-Navarrete R, Schwartz Z. Implant surface design regulates mesenchymal stem cell differentiation and maturation. Adv Dent Res. 2016;28(1):10–7. https://doi.org/10.1177/0022034515624444.View ArticlePubMedPubMed CentralGoogle Scholar
- Mamalis AA, Silvestros SS. Analysis of osteoblastic gene expression in the early human mesenchymal cell response to a chemically modified implant surface: an in vitro study. Clin Oral Implants Res. 2011;22(5):530–7. https://doi.org/10.1111/j.1600-0501.2010.02049. View ArticlePubMedGoogle Scholar
- Kato RB, Roy B, De Oliveira FS, Ferraz EP, De Oliveira PT, Kemper AG, et al. Nanotopography directs mesenchymal stem cells to osteoblast lineage through regulation of microRNA-SMAD-BMP-2 circuit. J Cell Physiol. 2014;229(11):1690–6. https://doi.org/10.1002/jcp.24614.View ArticlePubMedPubMed CentralGoogle Scholar
- Zhao G, Schwartz Z, Wieland M, Rupp F, Geis-Gerstorfer J, Cochran DL, et al. High surface energy enhances cell response to titanium substrate microstructure. J Biomed Mater Res A. 2005;74((1):49–58. https://doi.org/10.1002/jbm.a.30320.View ArticleGoogle Scholar
- Bang SM, Moon HJ, Kwon YD, Yoo JY, Pae A, Kwon IK. Osteoblastic and osteoclastic differentiation on SLA and hydrophilic modified SLA titanium surfaces. Clin Oral Implants Res. 2014;25(7):831–7. https://doi.org/10.1111/clr.12146.View ArticlePubMedGoogle Scholar
- Buser D, Broggini N, Wieland M, Schenk RK, Denzer AJ, Cochran DL, et al. Enhanced bone apposition to a chemically modified SLA titanium surface. J Dent Res. 2004;83(7):529–33. https://doi.org/10.1177/154405910408300704.View ArticlePubMedGoogle Scholar
- Gottlow J, Barkarmo S, Sennerby L. An experimental comparison of two different clinically used implant designs and surfaces. Clin Implant Dent Relat Res. 2012;14(Suppl 1):204–12. https://doi.org/10.1111/j.1708-8208.2012.00439. View ArticleGoogle Scholar
- Sartoretto SC, Alves AT, Resende RF, Calasans-Maia J, Granjeiro JM, Calasans-Maia MD. Early osseointegration driven by the surface chemistry and wettability of dental implants. J Appl Oral Sci. 2015;23(3):279–87. https://doi.org/10.1590/1678-775720140483.View ArticlePubMedPubMed CentralGoogle Scholar
- Lang NP, Salvi GE, Huynh-Ba G, Ivanovski S, Donos N, Bosshardt DD. Early osseointegration to hydrophilic and hydrophobic implant surfaces in humans. Clin Oral Implants Res. 2011;22(4):349–56. https://doi.org/10.1111/j.1600-0501.2011.02172. View ArticlePubMedGoogle Scholar
- Shanbhag S, Shanbhag V, Stavropoulos A. Genomic analyses of early peri-implant bone healing in humans: a systematic review. Int J Implant Dent. 2015;1(1):5. https://doi.org/10.1186/s40729-015-0006-2.View ArticlePubMedPubMed CentralGoogle Scholar
- Guler AU, Sumer M, Duran I, Sandikci EO, Telcioglu NT. Resonance frequency analysis of 208 Straumann dental implants during the healing period. J Oral Implantol. 2013;39(2):161–7. https://doi.org/10.1563/AAID-JOI-D-11-00060.View ArticlePubMedGoogle Scholar
- de Jesus RNR, Stavropoulos A, Oliveira MTF, Soares PBF, Moura CCG, Zanetta-Barbosa D. Histomorphometric evaluation of a dual acid-etched vs. a chemically modified hydrophilic dual acid-etched implant surface. An experimental study in dogs. Clin Oral Implants Res. 2017;28(5):551–7. https://doi.org/10.1111/clr.12833.View ArticlePubMedGoogle Scholar
- Frost HM. Skeletal structural adaptations to mechanical usage (SATMU): 1. Redefining Wolff’s law: the bone modeling problem. Anat Rec. 1990;226(4):403–13.View ArticlePubMedGoogle Scholar
- Berglundh T, Stavropoulos A; Working Group 1 of the VIII European Workshop on Periodontology. Preclinical in vivo research in implant dentistry. Consensus of the eighth European workshop on periodontology J Clin Periodontol 2012;39 Suppl 12:1–5. doi: https://doi.org/10.1111/j.1600-051X.2011.01827.
- Sawase T, Jimbo R, Baba K, Shibata Y, Ikeda T, Atsuta M. Photo-induced hydrophilicity enhances initial cell behavior and early bone apposition. Clin Oral Implants Res. 2008;19(5):491–6. https://doi.org/10.1111/j.1600-0501.2007.01509. View ArticlePubMedGoogle Scholar
- Ferguson SJ, Broggini N, Wieland M, de Wild M, Rupp F, Geis-Gerstorfer J, et al. Biomechanical evaluation of the interfacial strength of a chemically modified sandblasted and acid-etched titanium surface. J Biomed Mater Res A. 2006;78((2):291–7. https://doi.org/10.1002/jbm.a.30678.View ArticleGoogle Scholar
- Marin C, Granato R, Suzuki M, Gil JN, Piattelli A, Coelho PG. Removal torque and histomorphometric evaluation of bioceramic grit-blasted/acid-etched and dual acid-etched implant surfaces: an experimental study in dogs. J Periodontol. 2008;79(10):1942–9. https://doi.org/10.1902/jop.2008.080106.View ArticlePubMedGoogle Scholar
- Stadlinger B, Pourmand P, Locher MC, Schulz MC. Systematic review of animal models for the study of implant integration, assessing the influence of material, surface and design. J Clin Periodontol. 2012;39(Suppl 12):28–36. https://doi.org/10.1111/j.1600-051X.2011.01835. View ArticlePubMedGoogle Scholar
- Pearce AI, Richards RG, Milz S, Schneider E, Pearce SG. Animal models for implant biomaterial research in bone: a review. Eur Cell Mater. 2007;13:1):1–10.View ArticlePubMedGoogle Scholar
- Vasak C, Busenlechner D, Schwarze UY, Leitner HF, Munoz Guzon F, Hefti T, et al. Early bone apposition to hydrophilic and hydrophobic titanium implant surfaces: a histologic and histomorphometric study in minipigs. Clin Oral Implants Res. 2014;25(12):1378–85. https://doi.org/10.1111/clr.12277.View ArticlePubMedGoogle Scholar
- Bosshardt DD, Salvi GE, Huynh-Ba G, Ivanovski S, Donos N, Lang NP. The role of bone debris in early healing adjacent to hydrophilic and hydrophobic implant surfaces in man. Clin Oral Implants Res. 2011;22(4):357–64. https://doi.org/10.1111/j.1600-0501.2010.02107. View ArticlePubMedGoogle Scholar
- Kim S, Lee S, Cho I, Kim S, Kim T. Rotational resistance of surface-treated mini-implants. Angle Orthod. 2009;79(5):899–907. https://doi.org/10.2319/090608-466.1.View ArticlePubMedGoogle Scholar